# Epsilon Paper

date post

10-Oct-2014Category

## Documents

view

36download

2

Embed Size (px)

### Transcript of Epsilon Paper

CALPHAD 36 (2012) 16-22

Critical Assessment: MartensiteStart Temperature for the TransformationH.-S. Yang*, J. H. Jang*, H. K. D. H. Bhadeshia* and D. W. Suh*

*Graduate Institute of Ferrous Technology (GIFT) Pohang University of Science and Technology (POSTECH) Pohang 790-784, Republic of Korea of Cambridge Materials Science and Metallurgy Pembroke Street, Cambridge CB2 3QZ, U. K. University

AbstractIt is increasingly important in the context of highmanganese steels of the kind that lead to twinninginduced plasticity to be able to estimate the temperature at which martensite forms when austenite is cooled. We nd that the thermodynamic method used in similar calculations for martensite cannot in many cases be implemented because of apparently imprecise thermodynamic data, a conclusion partly validated using limited rstprinciples calculations. Alternative, empirical methods are also evaluated. The austenite grain size dependence of the martensitestart temperature has also been rationalised in terms of existing theory for martensite. Experiments have also been conducted to show that the problem in dealing with the martensite does not lie in the precision with which the transformation can be measured using dilatometry. Keywords: Martensite; thermodynamics; epsilon; start temperature; high Mn steels

1

Introduction

The basis for the calculation of the martensitestart (MS ) temperature was reviewed some time ago by Kaufman and Cohen [1]; martensite is triggered when the free energy change for transformation without a composition change (G ) reaches a critical value (GS ), the magnitude of which M is determined by stored energies and kinetic phenomena [2, 3]. Here refers to austenite and to bodycentred cubic or bodycentred tetragonal martensite. The method has been applied with some success to the transformation [412] and forms the basis of computer programs which take as inputs the thermodynamic parameters of the parent and product phases and output the 1

transformationstart temperature (for example, [13]). In this way, the incorporation of a previously excluded element on the MS temperature simply requires an understanding of how this element alters the thermodynamic stabilities of the phases involved. Iron in which the atoms are arranged on a hexagonal lattice is designated . Although this is not a common allotrope in alloyed iron at ambient pressure, it is gaining importance in lowcarbon, often low density, structural steels containing unconventionally large concentrations of manganese [1416]. It is also the basis of many ironbased shape memory alloys [1719]. The therefore features in reversible martensitic transformations and in steels where its transformation plasticity is exploited. It is important therefore, in the process of alloy design and optimisation, to be able to calculate its martensitestart temperature, at least as a function of the chemical composition. The last attempt at dealing with this issue was by Dogan and Ozer [20] who derived an empirical equation using linear regression analysis on some 17 ironbased alloys which undergo the martensitic transformation as follows: MS /K = 246 5.8wMn + 38.5wSi 61.5wCr 5.1wNi + 138wCe 146wTi 396wN (1)

where w represents the weight percent of the element identied in the subscript. The equation was derived for the concentration ranges 13.031.5Mn, 4.77.0Si, 011.6Cr, 06.8Ni wt%; Ce, Ti and N were each present in single alloys with values of 0.3, 0.6 and 0.3 wt% respectively. Standard errors were not quoted but the deviation from a t to this equation were typically less than 20 C. Dogan and Ozer also considered the use of thermodynamics as described above; however, neither the origin of the thermodynamic data nor the calculations of MS temperatures were presented in the paper, so it is not clear what was achieved. The purpose of the present work was to take a fresh look at this problem given the much larger availability of data due to the increased modern interest in low density and TRIP (transformation induced plasticity) steels based on the phase. To achieve this we have used a variety of empirical, thermodynamic and rstprinciples techniques.

2

Data

A search of the literature revealed a large number of sources of data [2078] which yielded some 328 combinations of chemical composition and martensitestart temperatures. The properties of the data are summarised in Table 1, and a spreadsheet containing the full details is available on [79]. The elements included C, Mn, Ni, Cr, Al, Si, Mo, Co, Cu, Nb, Ti, V and W. The data were subjected to multiple regression analysis to yield the following relationship which has a standard error of 26 K and a correlation coecient of 0.9: MS /K = 576 8 (489 31)wC (9.1 0.4)wMn (17.6 2)wNi (9.2 1)wCr (50 18)wNb (86 12)wTi (34 10)wV (13 5)wW +(21.3 2)wAl + (4.1 1)wSi (19.4 5)wMo (1 1)wCo (41.3 6)wCu

(2)

The extent of the t is illustrated in Fig. 1 and forms a rough method of estimating the martensite start temperature but the linear relationship and the implied lack of dependences between the 2

independent variables clearly cannot be justied. These particular issues are tackled later in the text when describing the neural network method, but a more fundamental approach would involve calculations based on phase stabilities which we address next.

3

Thermodynamic Calculations

By analogy with the transformation of austenite into martensite described in the introduction, the martensitestart temperature for martensite corresponds to that at which the driving force G achieves a critical value GS . Values of the driving force can in principle be calculated M using standard thermodynamic databases in combination with programs such as ThermoCalc or MTDATA. In the present work we used the TCFE6 database and ThermoCalc to produce the results illustrated in Fig. 2, which shows GS as a function of the measured transformationstart M temperatures obtained from the literature. The results are worrying in two respects; rst, that the driving force for a large number of alloys is positive, i.e., it is thermodynamically impossible for to form even though it is actually observed, and second, even when GS is negative, its M magnitude is in many cases very small and possibly insucient to account for the strain energy of transformation. There are two ways in which these results might be understood. The rst is that the experimental measurements of MS temperatures are faulty, but a detailed examination of the original sources of information indicated that any error in MS is much smaller than required to explain the sign and magnitude of the free energy change in cases where GS 0. Nevertheless, we discuss later in M this paper, our own experimental data designed to assess experimental error. The second and more likely explanation is that the database which forms the basis of the thermodynamic calculations described in section 3 is insuciently populated to represent martensite in concentrated alloys and at the relatively low temperatures involved. First principles calculations based on electron theory can be used to check this second explanation, but the calculations are expensive to conduct so a particular alloy which indicated a large positive G = G G in spite of the observation of martensite was selected for study. The conventional unit cells of austenite (FCC) and (HCP) can both be represented by the stacking of layers of closepacked planes, with each layer containing 4 atoms with a total of 24 atoms, and hence six layers, with both phases treated as being nonmagnetic. The lattice parameters (a, c) of the conventional hexagonal unit cell is then determined as a = 2a and c = 2 3a . The lattice parameter of austenite is applied as a = 3.59[80]. The only dierence between the FCC and A HCP forms is then the stacking sequence which is ABCABC and ABABAB, respectively. The alloy composition is created by an appropriate substitution of Fe atoms with ve Mn, two Si and two Cr atoms, Fig 3. The Kohn-Sham equation was solved self-consistently in terms of the total energy all-electron full-potential linearised augmented plane-wave method [81, 82] by using the generalised gradient approximation for the exchange-correlation potential. The integrations over the three dimensional Brillouin zone (3D-BZ) were calculated by the tetrahedron method over a 7 7 5 Monkhorst-Pack mesh [83], which corresponds to 123 k-points inside the irreducible wedge of 3D-BZ. The degree of 3

precision was obtained by considering a plane-wave cuto up to 21 Ry, which corresponds to about 3245 linearised augmented plane-waves per each k-point and spin. The wave functions, the charge densities, and the potential were expanded with l < 8 lattice harmonics inside each mun-tin sphere with a radius of 2.20 a.u. for Fe,Mn,Si and Cr. The density and potential in the interstitial region were depicted by using a star-function cuto at 340 Ry. Self-consistency was assumed when the root-mean-square distances between the input and output total charges were not more than 2.0 103 electrons/a.u.3 The sphere radii and Kmax within the whole lattice spacing range were kept constant, to keep the same degree of convergence for all the lattice constants studied. The transformation energies at 0 K and zero pressure were calculated to give G as 5.57 kJ mol1 and 3.49 kJ mol1 for the transformation in pure iron and 15Fe-5Mn-2Si-2Cr alloy respectively, where the alloy composition is expressed in terms of the number of atoms out of a total of 24 atoms. The value for pure iron is remarkably consistent with the 5.45 kJ mol1 reported in [84] for one atomsphere of pressure and 0 K. based on a thermodynamic assessment. This calculation proves the need for better thermodynamic data for use in software such as Thermocalc or MTDATA. It is

Recommended

*View more*